high-pressure dta studies of the phase behaviors of 4-n -butyl-thiocyanobiphenyl...
Post on 23-May-2018
Embed Size (px)
This work has been digitalized and published in 2013 by Verlag Zeitschrift fr Naturforschung in cooperation with the Max Planck Society for the Advancement of Science under a Creative Commons Attribution4.0 International License.
Dieses Werk wurde im Jahr 2013 vom Verlag Zeitschrift fr Naturforschungin Zusammenarbeit mit der Max-Planck-Gesellschaft zur Frderung derWissenschaften e.V. digitalisiert und unter folgender Lizenz verffentlicht:Creative Commons Namensnennung 4.0 Lizenz.
High-pressure DTA Studies of the Phase Behaviors of 4-n -butyl-thiocyanobiphenyl (4TCB) and 4-w-pentyl-4'-n-phenyl-cyanocyclohexane (5HCP) M. Massalska-Arod, A. Wrflinger3, and D. Bsinga
Institute of Nuclear Physics, 31-342 Krakow, Radzikowskiego 152, Poland a Institute of Physical Chemistry II, Ruhr-University, 44780 Bochum, Germany Reprint requests to Doc.dr hab. M. M-A.; Fax: 48-12-637-54-41.
Z. Naturforsch. 54a, 675-678 (1999); received November 5, 1999
DTA measurements of 4-/i-butyl-thiocyanobiphenyl (4TCB) and/?-cyano-/?'-pentylphenyl-cyclohex-ane (5HCP) have been performed in the temperature range 220 K-390 K and pressures up to 400 MPa. For 4TCP a transition from a crystalline to a liquid crystal phase (probably smectic E) could be detect-ed at higher pressures > 90 MPa. The pressure dependence of the transition temperature has been estab-lished. At pressures lower than 88.7 MPa no transition of SmE into a crystal or into a glass has been found. For 5HCP only the melting curve was observed, in contrast to 5PCH, which displays a liquid crystalline nematic phase.
Key words: DTA; High Pressures; Phase Transitions; Liquid Crystals.
The polymorphism of liquid crystalline (LC) materi-als can be studied using differential scanning calorime-try (DSC), differential thermal analysis (DTA), polariz-ing microscopy and dielectric relaxation spectroscopy [ 1 -3]. It was found that many liquid crystals exhibit pres-sure-induced disordered phases [2, 3]. For 4-n-butylthi-ocyanobiphenyl (4TCB) the DSC and polarizing micros-copy studies at normal pressure did not show any crys-tallization. Preliminary DSC measurements performed on heating allow to detect a very small anomaly at 218 K (the shape of which pointing rather to a glass tran-sition than to crystallization) and then a much higher peak at 356 K . The polarizing microscopy observations performed on cooling show at about 356 K the appear-ance of a texture typical for smectic E  which did not vanish down to liquid nitrogen temperatures. It was the aim of the pressure measurements (i) to find the condi-tions appropriate for the crystallization process and (ii)
a) c 4 H 9 Q Q N C S
b) C 5 H 1 1 < 0 > < 0 > C N
Fig. I. Chemical structure of a) butyl-thiocyanobiphenyl and b) cyano-pentylphenyl-cyclohexane.
to clarify the evidence for a glass transformation. In tum, for /?-cyano-p-pentylphenyl-cyclohexane (5HCP) no LC-phase has been observed at normal pressure . Therefore it should be checked, whether high-pressure DTA studies reveal new phase transitions.
The molecular structures of 4TCB and 5HCP are pre-sented in Figure 1. The 4TCB sample of 97% chemical purity was synthesized in the Military Technical Univer-sity (Warsaw, Poland) by Dabrowski. 5HCP was provid-ed by Prof. de Jeu (Amsterdam, The Netherlands). The high-pressure DTA studies have been carried out with the help of computer-assisted equipments described in . The measurements were performed in the temperature range from 220 K to 390 K on heating the sample at sev-eral pressures up to 400 MPa. To cover the whole pres-sure range two apparatus were used. In order to grow a crystal the sample was annealed during about 24 hours at several temperatures and pressures.
3. Results and Discussion
3.1 Butyl-thiocyanobiphenyl (4TCB)
In DTA measurements of 4TCB performed on heating at several pressures up to 110 MPa the anomaly con-
0932-0784 / 1200 / 0747-0001 $ 06.00 Verlag der Zeitschrift fr Naturforschung, Tbingen www.znaturforsch.com
676 M. Massalska-Arodz et al. High Pressure DTA Studies of 4TCB and 5HCP
nected with the smectic E - isotropic transition was ob-served. It was found that the transition temperatures in-crease linearly with pressure. In order to grow the crys-talline phase from the smectic E phase with the help of a higher pressure the sample was annealed during 24 hours at 233 K and 215 MPa. Then, on slow heating the sample, a second small anomaly was detected in the DTA curve at 335.3 K. Later the same feature was found for several pressures up to 400 MPa at higher transition temperatures. The anomaly was identified as being con-nected with a second transition from crystal into smec-tic E phase, as the values of the transition temperatures were much lower than those expected for the SmE-iso-tropic transformation. The next goal was to observe a DTA curve that reveals both anomalies at the same pres-sure. It was expected to be observed at lower tempera-tures; for higher pressures the clearing temperature is be-yond 390 K, which is the limit of the available tempera-ture range. Thus, the pressure was reduced slowly, and at 88.7 MPa the anomaly connected with Cr-SmE was observed at 306.5 K. Then the temperature was increased slowly, and at 385.2 K the second anomaly connected with the transition from SmE - isotropic was found at somewhat higher pressure, i.e. at 99.2 MPa. Figure 2 presents the DTA curve with these two anomalies. It was found that further reduction of the pressure does not re-sult in detection of the Cr-SmE transition, even after 24 hours of annealing. For pressures lower than 88.7 MPa the sample is still in the smectic E phase and may after supercooling transform into a glassy state as in polariz-ing microscopy observations at normal pressure. There a lowering of the temperature leads to a darkening of some parts of the microscopic image of the sample and to the appearance of fractures which disappear on heat-ing [1,4],
The phase behaviour under pressure is presented in Figure 3. The pressure dependence of the transition tem-peratures T(p) for the two phase transitions is well de-scribed by the following polynomials:
S m E-I : T( p)/K = 355.3 + 0.322 (p/MPa) -2 .0x 10^ (p/MPa)2,
Cr - SmE: T( p)/K = 285.2 + 0.238 (p/MPa) -0.46x IO-4 (p/MPa)2.
The detai Is of pressure and temperature conditions dur-ing annealing the sample are presented by squares and circles (explaining the starting conditions), and arrows showing the direction of changes. The dashed part of the lower line T(p) exhibits the range of pressure where the
T / K
Fig. 2. DTA traces for 4TCB showing anomalies due to Cr-SmE and SmE-1 transitions.
Fig. 3. Phase diagram for 4TCB established with DTA. Aste-risks show the data from DSC ,
sample exists in the smectic phase only. One can expect that below that T(p) the smectic phase can be super-cooled yielding a glass. There are two points marked by asterisks which show the transition temperatures (356 K and 218 K) observed in DSC at atmospheric pressure. The point with higher T, corresponding to SmE - isotrop-ic transition, coincides well with the result from the pres-sure studies. The point with small Flies definitely below the temperature which is extrapolated from the high pres-sure data. It seems that it corresponds rather to the tem-perature of transformation between the SmE phase and a glass G. DSC studies at atmospheric pressure with a scanning rate of 10 K/min detect the transition as a very small anomaly on cooling at 215 K and at heating at 218 K. Detailed description of the SmE-G transforma-tion requires further studies. Although many different thermal treatments have been employed, it was not pos-
M. Massalska-Arodz et al. High Pressure DTA Studies of 4TCB and 5HCP
Table 1. Thermodynamic properties of 4TCB. 360
Phase T Enthalpy Entropy Volume AT/Ap transitions [K1 AH AS AV
[kJ/mol] [J/mol K] [cnv/mol] [K/MPa]
SmE-Isotrop 355.3 12.09 34.0 10.96 0.332 C r - S m E 285.2 3.8 13.4 3.2 0.238
sible to observe the crystallization at normal pressure. Obviously high pressure favours the transformation to the crystal phase that has also been observed in previous studies on disordered molecular crystals .
In Table 1 the thermodynamic data for 4TCB estimat-ed for phase transitions at atmospheric pressure.
The volume changes AV for SmE-I were estimated using the Clausius-Clapeyron equation. The transition enthalpy AH = 3.8 kJ/mol for the Cr-SmE transition (not observed at atmospheric pressure) was estimated from the ratio of the transition enthalpies at 88.7 MPa, i.e. 1 : 3.2, assuming that it is independent of the pres-sure. The same procedure was used for the calculation of the entropy and volume changes.
4TCB displays no nematic phase. Thus, it seems clear that the melting is connected with much smaller chang-es on the molecular level of the sample than the transi-tion at the clearing point, in accordance with the ratio of the enthalpy changes. In the so-called low-temperature smectic E phase the 3-d positional order of the centers of gravity of 4TCB molecules as well as the long range orientational order of long molecular axes does not dif-fer much from the case of the true crystal. During melt-ing the molecules gain only a freedom of ^-rotation and thus the ability of the direction of the long axes, while at the clearing point both the 3-d positional and orienta-tional order is lost. The small AH, AS, and A V values at melting and the large AH, AS, and A V values at the clear-ing point reflect the relation between the magnitudes of those changes. Contrary to that for liquid crystalline ma-terials possessing the nematic phase, the enthalpy chang-es